The SMSI Effect in the System Rh/Ti02 at High Metal Loading
Noble metal catalysts on certain supports such as Ti02, V205, Nb205, exhibit a significant depression of hydrogen and CO chemisorption after reduction at temperatures higher than 700 K, without remarkable sintering of the metal particles (1). This socalled SMSI effect (strong metal-support interaction) has a strong influence on the catalytic properties. Vannice reported on a higher activity of the catalysts in the SMSI state for CO hydrogenation and on an improved selectivity to higher hydrocarbons (24). On the other hand, for the reactions such as hydrogenation and hydrogenolysis of hydrocarbons a significant decrease of activity has been found in the SMSI state (5-8). In our investigation we studied the properties of 5 wt% Rh/TiOz catalysts in connection with SMSI, and found a depression due to the SMSI effect not only in the chemisorption of H2, but also the activity of the hydrogenation of CO (9). In the present study, the influence of metal loading in the Rh/TiOz system on the SMSI behavior was investigated. Our main interest dealt with the consumption of hydrogen during the SMSI formation by hightemperature reduction and with the dependence of the depression of chemisorption on the metal loading and particle size. Therefore we prepared catalysts with 25 and 60 wt% Rh on TiOz (anatase) and examined the Hz chemisorption as well as the catalytic activity of CO-HZ reaction on these catalysts after definite pretreatments. In this note, we report on the formation of the SMSI state and the chemisorption of hydrogen. The results of the catalytic experiments will be reported elsewhere (10).
The catalysts were prepared by impregnating the support TiOz (Aerosil P-25, 50 m2/g) with an aqueous solution of RhC& * 3H20 and subsequent drying on air at 383 K. The pretreatment of the catalysts, the adsorption and reaction measurements were performed in a closed gas circulation system with a liquid-nitrogen cold trap. The pretreatments included reduction with hydrogen at low temperature (573 K) and calcination with oxygen at 723 K. To generate the SMSI state the catalysts were reduced with hydrogen at 723 K overnight after the low-temperature reduction. The amounts of consumed hydrogen or oxygen during the pretreatment were measured volumetrically. Adsorption measurements were carried out at room temperature with 150-200 Torr of H2 and waited until no more uptake was observed (about 1 h). RESULTS
Table I shows the results of the hydrogen adsorption on the catalysts after reduction at low temperature (LTR) and in the SMSI state. For each sample several cycles of reduction at low and high temperatures and calcination were performed. It is evident from this table that the dispersion decreased after the first cycle but remained unchanged then at the stable value. Similar results were obtained by Sexton et al. (II) by XPS experiments on Rh/TiOz catalysts. The LTR data show that the dispersion of Rh in the 25% sample is higher if the catalyst is first calcined in oxygen and then reduced, probably because of the better fixing
300 0021-9517/M $3.00 Copyright All rights
0 1985 by Academic Press, Inc. of reproduction in any form reserved.
NOTES TABLE 1 Chemisorption and Consumption of Hz on Rh/TiOr Catalysts (cm3 (STP)/g-Rh) Catalysts
Treatments temp. (K)
LTR Hz ads. W-W
SMSI Hz ads. W-W
Ratio of Hz ads. on SMSVLTR
H2 cons. (red. 732 K)
H2 cons. H2 ads (LTR)
25 wt% (first calcination)
16.q0.15) 12.9(0.12) 13.5(0.12)
12.7(0.12) 8.6(0.08) 8.4(0.08)
O.ll(O.008) 1.1(0.010) 1.4(0.013)
0.07 0.13 0.17
OzCW, &(573) 25 wt% (first reduced) 6OWt%
HdS73) o&‘=), &(573)
of the initial dispersity by the calcination. The data for the catalysts in the SMSI state show that the amount of the chemisorbed hydrogen is reduced significantly in all cases. It is remarkable that even in the case of 60 wt% Rh/TiOz we could observe a SMSI behavior after the reduction at 723 K. The extent of depression of hydrogen adsorption actually decreased with increasing particle size (the ratio SMSULTR increases), but even with 60 wt% Rh/TiOz catalyst this depression of hydrogen adsorption is significant. In this context it is interesting to mention the results obtained by Sexton et al. (II), who have shown by TPR that even in a mixture of Pt powder with TiOz, the TiOz is reduced at temperatures between 673 and 773 K, whereas pure TiOz is reduced at above 823 K. In all cases, the normal state could be obtained again by the treatment with 02 at 723 K and subsequent reduction at 573 K (Table 1). In the case of 60 wt% Rh/TiOz this reoxidation was very slow. It requires 10 days to reach 80% reoxidation whereas only a few hours were sufficient in other cases. Here the situation is similar to the observation of Foger et al. (6) for the Ir/ TiOz system, in that the catalysts with a lower dispersion (~0.1) need to be under more severe conditions (higher temperatures) for reoxidation. As already mentioned we estimated the
amount of hydrogen consumed during the reduction at higher temperature (723 K) required to produce the SMSI state. This consumption was measured after reduction at 573 K, HZ chemisorption, and subsequent evacuation at 573 K. The corresponding figures are shown in Table 1. As a product of the reduction at higher temperatures, water was detected by gas chromatography in an amount which approximately corresponds to the consumed hydrogen. The ratio between the amount of hydrogen consumed and that chemisorbed after LTR is constant for each sample.- The plots of this ratio result in a very good correlation (Fig. 1)
FIG. 1. The relationship between the amount of hydrogen consumed during high-temperature reduction (HTR) and the amount of hydrogen chemisorbed after low-temperature reduction (LTR). (0) 25 wt%, first calcined; (0) 25 wt%, first reduced; (A) 60 wt%.
NOTES with a slope of 1.7 (20.1) and intersection Fung, S. C., Baker, R. T. K., and Horsley, J. A., Science 211, 1121 (1981). of the abscissa at 2.6 (k1.4) cm3 (STP) HZ/ g-Rh. According to these data a small 2. Vannice, M. A., and Garten, R. L., U.S. Patent 4,116,994 (1978). amount of hydrogen, which corresponded 3. Vannice, M. A., and Garten, R. L., .I. Catal. 56, to approximately 2% of the Rh content, is 236 (1979). consumed independently of the Rh surface 4. Vannice, M. A., J. Catal. 74, 199 (1982). atoms whereas the main part of hydrogen is 5. Meriaudeau, P., Ellestad, 0. H., Defaux, M., and Naccache, C., J. Catal. 75, 243 (1982). related to the chemisorbed hydrogen by a Foger, K., J. Catal. 78, 406 (1982). factor of 1.7. The actual meaning of these 6.7. Turlier, P., and Martin, G. A., React. Kinet. Cafigures is not quite clear at present and tal. Lett. 21, 387 (1982). needs further investigation, but there seems 8. Burch, R., and Flambard, A. R., J. Catal. 78,389 (1982). to be proof that there is a connection be9. Orita, H., Naito, S., and Tamaru, K., J. Chem. tween the amount of metal atoms exposed Sot. Chem. Commun., 993 (1983). and the amount of hydrogen consumed dur- 10. Miessner, H., Orita, H., Naito, S., and Tamaru, ing formation of the SMSI state. A plausiK., in preparation. ble explanation of these results is that Ti02 II. Sexton, B. A., Hughes, A. E., and Foger, K., J. Catal. 77, 85 (1982). around Rh metal particles is reduced by hy12. Kunimori, K., Matsui, S., and Uchijima, T., J. drogen to form water, whose amount may Catal. 85, 253 (1984). be proportional to the surface area of Rh 13. Imelik, B., Naccache, C., Coudurier, G., Prametal. liaud, H., Meriaudeau, P., Gallezot, P., Martin, Our results apparently support the recent G. A., and Verbrine, J. C., Stud. Su$. Sci. Catal. 11, 95 (1982). view that SMSI is caused by migration of reduced TiO, (1 < x < 2) on the metal sur- 14. Resasco, D. E., and Haller, G. L., J. Catal. 82, 297 (1983). faces (U-17), because of the good correla- 15. Jiang, Xuan-Zhen, Hayden, T. F., and Dumesic, tion between the amount of the surface J. A., J. Catal. 83, 168 (1983). metal atoms and the amount of hydrogen 16. Cairns, J. A., Baglin, J. E. E., and Ziegler, J. F., J. Catal. 83, 301 (1983). consumption during the high-temperature reduction of 1 wt% Pt/Ti02. They found a 17. Sadegli, H. R., and Henrich, V. E., J. Catal. 87, 279 (1984). linear correlation between the amount of consumed hydrogen and the decrease of H2 H. MIESSNER~ chemisorption in the SMSI state. From S. NAITO* their work it is possible to estimate the ratio K. TAMARU of consumed hydrogen to chemisorbed hydrogen after reduction at 473 K to be from 2 Department of Chemistry to 4. This is in qualitatively good agreement Faculty of Science with our results and also supports the idea The University of Tokyo of a connection between the metal surface Hongo, Bunkyo-ku, Tokyo, 113, Japan and the consumed hydrogen during highReceived August 29, 1984 temperature reduction. REFERENCES 1. Tauster, S. J., Fung, S. C., and Garten, R. L., J. Amer. Chem. Sot. 100, 170 (1978); Tauster, S. J.,
’ Permanent address: Central Institute of Physical Chemistry, The Academy of Science of the GDR, Rudower Chaussee 5, 1199 Berlin, GDR. z To whom correspondence should be addressed.